**A. Appendix 121**

**A.4. Convergence tests and BSSE corrections for cluster calculations**

A.4. Convergence tests and BSSE corrections for cluster calculations neutral F center (formed in the center of the cluster) was calculated for increasing shells of em-bedding point charges. This was performed for two different emem-bedding geometries, spherical and cubic. Fig.A.6shows that the formation energy converges fast with respect to the number of embedding shells and that the formation energy does not depend on the embedding geometry.

The calculations were performed using PBE exchange-correlation treatment.

**Figure A.6.: Convergence of formation energy**G^{0}_{f} for F^{0}in eV with respect to number of point
charge embedding shells, calculated with PBE, basis set superposition error has been removed.

a) cube-shaped embedding , b) spherical embedding

For comparison, the formation energies of the F^{0} center, as calculated with different methods
using the embedded Mg6O9 cluster, are shown in TableA.3. A tier 3 basis set was used for
all atoms in calculations with FHI-aims, whereG^{0}_{f} is converged within 0.05 eV for all methods
shown. TURBOMOLE calculations were performed by S. Sicolo (Humboldt University Berlin).

All formation energies were corrected for the basis set superposition error (BSSE) using the Boys-Bernardi counterpoise correction [198]. The BSSE may arise due to the incompleteness of the atom centered orbital basis sets used in the calculations [99,103,198,247]. Depending on the geometric structure and the basis set used, overlap of basis functions can improve the computed total energy of a system. When energy differences between systems with different numbers of atoms or different atomic arrangements are considered, this may lead to an error, since the superposition of wave functions is not the same for the different atomic configurations.

For the defect formation energyG^{0}_{f} three systems are calculated – the cluster without defect, the
cluster with defect, and a bare oxygen atom. For example, in the full cluster the atoms adjacent
to the central oxygen atom might profit from its basis functions, while this is not the case,
when the central oxygen atom is removed in the cluster with a defect. The BSSE corrections as
obtained with FHI-aims for the vertical formation energiesG^{0}_{f} for an F^{0}center, calculated in the
embedded Mg6O9 cluster, are shown in TableA.4. In general, the BSSE for GGA and hybrid
functional ground state energies is small when computed with FHI-aims, due to the construction
of numeric atom-centered basis sets, where the total energy of a free non-spinpolarized atom is

A.4. Convergence tests and BSSE corrections for cluster calculations
already converged at the minimum basis set level [99]. For explicitly correlated methods also
unoccupied orbitals are needed (see Sec. 2), so that the BSSE becomes severe [103]. Using
the counterpoise correction method, the BSSE can be obtained and corrected for (G^{0}_{f} → G^{0}_{f} +

∆^{CP}(G^{0}_{f})) by computing the system fragments, here the cluster with a defectE_{F}^{CP}0 and the bare
oxygen atom,E_{Oatom}^{CP} ), with the same basis functions that are used in the full system (here the
pristine cluster) [198],

∆^{CP}(G^{0}_{f}) =E_{F}^{CP}0 +E_{O atom}^{CP} −(E_{F}^{0} +E_{O atom}).

Indeed, as shown in Table A.4, the absolute values of the BSSE corrections to the formation
energiesG^{0}_{f} are negligible (<0.04 eV) for the GGA functional PBE, and the hybrid functionals
HSE06, PBE0, and B3LYP, while for the explicitly correlated methods MP2 and RPA they are
as large as 1.71 eV and 2.75 eV, respectively. For all cluster calculations in this work,
BSSE-corrected energies were used for consistency when comparing different methods and formation
energies calculated with different codes. In general, the BSSE also concerns periodic
calcu-lations. Since based on the cluster results its absolute value is assumed to be< 0.04 eV for
the GGA and hybrid DFT defect formation energy calculations performed in this work, it was
neglected in these calculations.

**Table A.3.: Vertical formation energies** G^{0}_{f} for F^{0} in eV, as obtained from embedded Mg_{6}O_{9}
cluster calculations (incl. BSSE corrections).

Code PBE HSE06 PBE0 B3LYP MP2 RPA CCSD(T)

@PBE

TURBO- 7.18 – 7.02 7.37 – – 7.09

MOLE

FHI-aims 7.11 7.03 6.99 7.35 8.05 7.13 –

**Table A.4.: Basis set superposition corrections**∆^{CP}_{G}0
f

in eV, as obtained from embedded Mg_{6}O_{9}
*cluster calculations with FHI-aims (see text), using tier 3 basis sets and really tight/safe grid*
settings.

PBE HSE06 PBE0 B3LYP MP2 RPA@PBE

-0.03 -0.03 -0.03 -0.04 -1.71 -2.75

**Bibliography**

[1] Z. Zhan, J. Chen, S. Guan, L. Si, and P. Zhang, “Highly sensitive and thermal stable CO
gas sensor based on SnO2 modified by SiO2*,” J. Nanosci. Nanotechnol., vol. 13, no. 2,*
pp. 1507–1510, 2013.

*[2] T. H. Maiman, “Stimulated optical radiation in ruby,” Nature, vol. 187, pp. 493–494,*
1960.

[3] S. Kumar, N. K. Verma, and M. L. Singla, “Study on reflectivity and photostability of
Al-doped TiO_{2}*nanoparticles and their reflectors,” J. Mater. Res., vol. 28, no. 03, pp. 521–*

528, 2013.

[4] M. A. El-Gammal, A. M. El-Alfy, and N. M. Mohamed, “Using magnesium oxide
*wall-board as an alternative building façade cladding material in modern cairo buildings,” J.*

*Appl. Sci. Res., vol. 8, no. 4, pp. 2024–2032, 2012.*

[5] M. A. Mitchnick, D. Fairhurst, and S. R. Pinnell, “Microfine zinc oxide (Z-Cote) as a
*photostable UVA/UVB sunblock agent,” J. Am. Acad. Dermatol., vol. 40, pp. 85–90,*
1999.

[6] H. Jiang, J. Ma, and C. Li, “Mesoporous carbon incorporated metal oxide nanomaterials
*as supercapacitor electrodes,” Adv. Mater., vol. 24, no. 30, p. 4196, 2012.*

[7] A. Fujishima and K. Honda, “Electrochemical photolysis of water at a semiconductor
*electrode,” Nature, vol. 238, pp. 37–38, 1972.*

*[8] A. Fujishima, T. N. Rao, and D. A. Tryk, “Titanium dioxide photocatalysis,” J. *
*Pho-tochem. Photobiol. C: PhoPho-tochem. Rev., vol. 1, pp. 1–21, 2000.*

[9] S. U. M. Khan, M. Al-Shahry, and W. B. Ingler, “Efficient photochemical water splitting
by a chemically modified n-TiO_{2}*,” Science, vol. 297, pp. 2243–2245, 2002.*

[10] M. Ni, M. K. Leung, D. Y. Leung, and K. Sumathy, “A review and recent developments in
*photocatalytic water-splitting using for hydrogen production,” Renew. Sust. Energ. Rev.,*
vol. 11, pp. 401–425, 2007.

[11] T. Ito and J. H. Lunsford, “Synthesis of ethylene and ethane by partial oxidation of
*methane over lithium-doped magnesium oxide,” Nature, vol. 314, pp. 721–722, 1985.*

[12] T. Ito, J. Wang, C. H. Lin, and J. H. Lunsford, “Oxidative dimerization of methane over
*a lithium-promoted magnesium oxide catalyst,” J. Am. Chem. Soc., vol. 107, pp. 5062–*

5068, 1985.

Bibliography [13] E. Iwamatsu, T. Moriyama, N. Takasaki, and K. Aika, “Oxidative coupling of methane

over Na^{+}- and Rb^{+}*-doped MgO catalysts,” J. Catal., vol. 113, pp. 25–35, 1988.*

[14] V. Sokolovskii, S. Aliev, O. Buyevskaya, and A. Davydov, “Type of hydrocarbon
acti-vation and nature of active sites of base catalysts in methane oxidative
*dehydrodimeriza-tion,” Catal. Today, vol. 4, pp. 293–300, 1989.*

[15] G. J. Hutchings, M. S. Scurrell, and J. Woodhouse, “Oxidative coupling of methane using
*Li/MgO catalyst: Re-appraisal of the optimum loading of Li,” Catal. Lett., vol. 5, pp. 301–*

308, 1990.

[16] V. R. Choudhary, V. H. Rane, and S. T. Chaudhari, “Influence of various promoters on the
*basicity and catalytic activity of MgO catalysts in oxidative coupling of methane,” Catal.*

*Lett., vol. 6, pp. 95–98, 1990.*

[17] G. Hoogendam, K. Seshan, J. van Ommen, and J. Ross, “Oxidative coupling of methane
*over doped Li/MgO catalysts,” Catal. Today, vol. 21, pp. 333–340, 1994.*

[18] R. Nibbelke, J. Scheerova, M. Decroon, and G. Marin, “The oxidative coupling of methane over MgO-based catalysts: A steady-state isotope transient kinetic analysis,”

*J. Catal., vol. 156, pp. 106–119, 1995.*

[19] R. L. P. Goncalves, F. C. Muniz, F. B. Passos, and M. Schmal, “Promoting effect of Ce
*on the oxidative coupling of methane catalysts,” Catal. Lett., vol. 135, pp. 26–32, 2010.*

[20] L. Tang, D. Yamaguchi, L. Wong, N. Burke, and K. Chiang, “The promoting effect of
*ceria on Li/MgO catalysts for the oxidative coupling of methane,” Catal. Today, vol. 178,*
pp. 172–180, 2011.

[21] K. Langfeld, B. Frank, V. E. Strempel, C. Berger-Karin, G. Weinberg, E. V. Kondratenko,
and R. Schomäcker, “Comparison of oxidizing agents for the oxidative coupling of
*methane over state-of-the-art catalysts,” Appl. Catal. A, vol. 417–418, pp. 145–152, 2012.*

[22] Q. Wu and R. van de Krol, “Selective photoreduction of nitric oxide to nitrogen by
nanos-tructured TiO_{2}*photocatalysts: Role of oxygen vacancies and iron dopant,” J. Am. Chem.*

*Soc., vol. 134, pp. 9369–9375, 2012.*

[23] G. Makov and M. C. Payne, “Periodic boundary conditions in ab initio calculations,”

*Phys. Rev. B, vol. 51, pp. 4014–4022, 1995.*

[24] C. Weinert and M. Scheffler, “Chalcogen and vacancy pairs in silicon: Electronic structure
*and stabilities,” Mater. Sci. Forum, vol. 10–12, pp. 25–30, 1986.*

*[25] J. Rogal and K. Reuter, Ab Initio Atomistic Thermodynamics for Surfaces: A Primer.*

Neuilly-sur-Seine, 2007.

[26] L. A. Kappers, R. L. Kroes, and E. B. Hensley, “F^{+}and F’ centers in magnesium oxide,”

*Phys. Rev. B, vol. 1, pp. 4151–4157, 1970.*

Bibliography [27] L. Kantorovich, J. Holender, and M. Gillan, “The energetics and electronic structure of

*defective and irregular surfaces on MgO,” Surf. Sci., vol. 343, pp. 221–239, 1995.*

[28] Z. Yang, R. Wu, Q. Zhang, and D. W. Goodman, “Adsorption of Au on an O-deficient
*MgO(001) surface,” Phys. Rev. B, vol. 65, p. 155407, 2002.*

[29] J. Carrasco, N. Lopez, and F. Illas, “First principles analysis of the stability and diffusion
*of oxygen vacancies in metal oxides,” Phys. Rev. Lett., vol. 93, p. 225502, 2004.*

[30] E. Scorza, U. Birkenheuer, and C. Pisani, “The oxygen vacancy at the surface and in bulk
*MgO: an embedded-cluster study,” J. Chem. Phys., vol. 107, pp. 9645–9658, 1997.*

[31] J.-L. Dubois and C. J. Cameron, “Common features of oxidative coupling of methane
*cofeed catalysts,” Appl. Catal., vol. 67, no. 1, pp. 49–71, 1990.*

[32] I. Balint and K.-i. Aika, “Specific defect sites creation by doping MgO with lithium and
*titanium,” Applied Surf. Sci., vol. 173, pp. 296–306, 2001.*

*[33] M. Born and R. Oppenheimer, “Zur Quantentheorie der Molekeln,” Ann. Phys., vol. 389,*
pp. 457–484, 1927.

[34] H. Hellmann, “Zur Rolle der kinetischen Elektronenenergie für die zwischenatomaren
*Kräfte,” Z. Phys. A - Hadron Nucl., vol. 85, no. 3, pp. 180–190, 1933.*

[35] D. R. Hartree, “The wave mechanics of an atom with a non-Coulomb central field. Part I.

*Theory and methods,” Math. Proc. Cambridge Philos. Soc., vol. 24, no. 01, pp. 89–110,*
1928.

[36] W. Ritz, “Über eine neue Methode zur Lösung gewisser Variationsprobleme der
*mathe-matischen Physik.,” J. reine angew. Math., no. 135, pp. 1–61, 1909.*

*[37] P. Hohenberg and W. Kohn, “Inhomogeneous electron gas,” Phys. Rev., vol. 136,*
pp. B864–B871, 1964.

*[38] L. H. Thomas, “The calculation of atomic fields,” Math. Proc. Cambridge Philos. Soc.,*
vol. 23, no. 05, pp. 542–548, 1927.

[39] E. Fermi, “Eine statistische Methode zur Bestimmung einiger Eigenschaften des Atoms
*und ihre Anwendung auf die Theorie des periodischen Systems der Elemente,” Z. Phys.,*
vol. 48, pp. 73–79, 1928.

*[40] E. K. U. Gross and R. M. Dreizler, Density Functional Theory. Springer, 1995.*

[41] M. Levy, “Universal variational functionals of electron densities, first-order density
*matri-ces, and natural spin-orbitals and solution of the v-representability problem,” Proc. Natl.*

*Acad. Sci., vol. 76, pp. 6062–6065, 1979.*

[42] W. Kohn and L. J. Sham, “Self-consistent equations including exchange and correlation
*effects,” Phys. Rev., vol. 140, pp. A1133–A1138, 1965.*

Bibliography
[43] M. Levy, J. P. Perdew, and V. Sahni, “Exact differential equation for the density and
*ionization energy of a many-particle system,” Phys. Rev. A, vol. 30, pp. 2745–2748, 1984.*

[44] C.-O. Almbladh and U. von Barth, “Exact results for the charge and spin
*densi-ties, exchange-correlation potentials, and density-functional eigenvalues,” Phys. Rev. B,*
vol. 31, pp. 3231–3244, 1985.

[45] J. F. Janak, “Proof that∂E/∂ni =ε*in density-functional theory,” Phys. Rev. B, vol. 18,*
pp. 7165–7168, 1978.

[46] T. Koopmans, “Über die Zuordnung von Wellenfunktionen und Eigenwerten zu den
*einzelnen Elektronen eines Atoms,” Physica, vol. 1, no. 1–6, pp. 104–113, 1934.*

*[47] J. C. Slater, Quantum Theory of Molecules and Solids Vol. 4: The Self-Consistent Field*
*for Molecules and Solids. International Series in Pure and Applied Physics, New York:*

McGraw-Hill, 1 ed., 1974.

*[48] P. A. M. Dirac, “Note on exchange phenomena in the Thomas atom,” Math. Proc. *
*Cam-bridge, vol. 26, no. 03, pp. 376–385, 1930.*

[49] D. M. Ceperley and B. J. Alder, “Ground state of the electron gas by a stochastic method,”

*Phys. Rev. Lett., vol. 45, pp. 566–569, 1980.*

[50] J. P. Perdew and Y. Wang, “Accurate and simple analytic representation of the
*electron-gas correlation energy,” Phys. Rev. B, vol. 45, pp. 13244–13249, 1992.*

[51] R. O. Jones and O. Gunnarsson, “The density functional formalism, its applications and
*prospects,” Rev. Mod. Phys., vol. 61, pp. 689–746, 1989.*

[52] J. P. Perdew, K. Burke, and M. Ernzerhof, “Generalized gradient approximation made
*simple,” Phys. Rev. Lett., vol. 77, pp. 3865–3868, 1996.*

*[53] E. H. Lieb and S. Oxford, “Improved lower bound on the indirect Coulomb energy,” Int.*

*J. Quantum Chem., vol. 19, no. 3, pp. 427–439, 1981.*

[54] V. N. Staroverov, G. E. Scuseria, J. Tao, and J. P. Perdew, “Tests of a ladder of density
*functionals for bulk solids and surfaces,” Phys. Rev. B, vol. 69, p. 075102, 2004.*

[55] F. Tran, R. Laskowski, P. Blaha, and K. Schwarz, “Performance on molecules, surfaces,
*and solids of the Wu-Cohen GGA exchange-correlation energy functional,” Phys. Rev. B,*
vol. 75, p. 115131, 2007.

[56] V. N. Staroverov, G. E. Scuseria, J. Tao, and J. P. Perdew, “Erratum: Tests of a ladder of
*density functionals for bulk solids and surfaces [Phys. Rev. B 69, 075102 (2004)],” Phys.*

*Rev. B, vol. 78, p. 239907, 2008.*

*[57] W. Koch and M. C. Holthausen, A Chemist’s Guide to Density Functional Theory. John*
Wiley & Sons, 2000.

Bibliography
*[58] A. D. Becke, “A new mixing of Hartree–Fock and local density-functional theories,” J.*

*Chem. Phys., vol. 98, pp. 1372–1377, 1993.*

*[59] A. D. Becke, “Density-functional thermochemistry. III. The role of exact exchange,” J.*

*Chem. Phys., vol. 98, pp. 5648–5652, 1993.*

*[60] H. J. Monkhorst, “Hartree-Fock density of states for extended systems,” Phys. Rev. B,*
vol. 20, pp. 1504–1513, 1979.

[61] J. Delhalle and J.-L. Calais, “Direct-space analysis of the Hartree-Fock energy bands and
*density of states for metallic extended systems,” Phys. Rev. B, vol. 35, pp. 9460–9466,*
1987.

[62] J. Paier, M. Marsman, and G. Kresse, “Why does the B3LYP hybrid functional fail for
*metals?,” J. Chem. Phys., vol. 127, p. 024103, 2007.*

[63] J. Heyd, G. E. Scuseria, and M. Ernzerhof, “Hybrid functionals based on a screened
*Coulomb potential,” J. Chem. Phys., vol. 118, pp. 8207–8215, 2003.*

[64] J. P. Perdew, M. Ernzerhof, and K. Burke, “Rationale for mixing exact exchange with
*density functional approximations,” J. Chem. Phys., vol. 105, pp. 9982–9985, 1996.*

[65] A. V. Krukau, O. A. Vydrov, A. F. Izmaylov, and G. E. Scuseria, “Influence of the
*ex-change screening parameter on the performance of screened hybrid functionals,” J. Chem.*

*Phys., vol. 125, p. 224106, 2006.*

[66] K. Kim and K. D. Jordan, “Comparison of density functional and MP2 calculations on
*the water monomer and dimer,” J. Phys. Chem., vol. 98, pp. 10089–10094, 1994.*

[67] C. Møller and M. S. Plesset, “Note on an approximation treatment for many-electron
*systems,” Phys. Rev., vol. 46, pp. 618–622, 1934.*

*[68] A. Szabo and N. S. Ostlund, Modern Quantum Chemistry: Introduction to Advanced*
*Electronic Structure Theory. Courier Dover Publications, 1989.*

[69] D. Bohm and D. Pines, “A collective description of electron interactions. I. Magnetic
*interactions,” Phys. Rev., vol. 82, pp. 625–634, 1951.*

[70] D. Pines and D. Bohm, “A collective description of electron interactions: II. Collective vs
*individual particle aspects of the interactions,” Phys. Rev., vol. 85, pp. 338–353, 1952.*

[71] D. Bohm and D. Pines, “A collective description of electron interactions: III. Coulomb
*interactions in a degenerate electron gas,” Phys. Rev., vol. 92, pp. 609–625, 1953.*

[72] X. Ren, P. Rinke, C. Joas, and M. Scheffler, “Random-phase approximation and its
*applications in computational chemistry and materials science,” J. Mater. Sci., vol. 47,*
pp. 7447–7471, 2012.

*[73] D. Langreth and J. Perdew, “The exchange-correlation energy of a metallic surface,” Solid*
*State Commun., vol. 17, pp. 1425–1429, 1975.*

Bibliography
[74] O. Gunnarsson and B. I. Lundqvist, “Exchange and correlation in atoms, molecules, and
*solids by the spin-density-functional formalism,” Phys. Rev. B, vol. 13, pp. 4274–4298,*
1976.

[75] D. C. Langreth and J. P. Perdew, “Exchange-correlation energy of a metallic surface:

*Wave-vector analysis,” Phys. Rev. B, vol. 15, pp. 2884–2901, 1977.*

*[76] R. Kubo, “The fluctuation-dissipation theorem,” Rep. Prog. Phys., vol. 29, no. 1, pp. 255–*

284, 1966.

[77] F. Furche, “Molecular tests of the random phase approximation to the
*exchange-correlation energy functional,” Phys. Rev. B, vol. 64, p. 195120, 2001.*

[78] J. Harl and G. Kresse, “Accurate bulk properties from approximate many-body
*tech-niques,” Phys. Rev. Lett., vol. 103, p. 056401, 2009.*

[79] X. Ren, A. Tkatchenko, P. Rinke, and M. Scheffler, “Beyond the random-phase
*approx-imation for the electron correlation energy: The importance of single excitations,” Phys.*

*Rev. Lett., vol. 106, p. 153003, 2011.*

[80] K. S. Singwi, M. P. Tosi, R. H. Land, and A. Sjölander, “Electron correlations at metallic
*densities,” Phys. Rev., vol. 176, pp. 589–599, 1968.*

*[81] A. L. Fetter and J. D. Walecka, Quantum Theory of Many-Particle Systems. Courier Dover*
Publications, 1971.

*[82] A. A. Abrikosov and L. P. Gorkov, Methods of Quantum Field Theory in Statistical*
*Physics. Courier Dover Publications, 1975.*

[83] L. Hedin, “New method for calculating the one-particle Green’s function with application
*to the electron-gas problem,” Phys. Rev., vol. 139, pp. A796–A823, 1965.*

[84] W. G. Aulbur, L. Jönsson, and J. W. Wilkins, “Quasiparticle calculations in solids,” in
*Solid State Physics (Henry Ehrenreich and Frans Spaepen, eds.), vol. 54, pp. 1–218, *
Aca-demic Press, 1999.

[85] G. Onida, L. Reining, and A. Rubio, “Electronic excitations: Density-functional versus
*many-body Green’s–function approaches,” Rev. Mod. Phys., vol. 74, pp. 601–659, 2002.*

[86] V. Galitskii and A. Migdal, “Application of quantum field theory methods to the many
*body problem,” Sov. Phys. JETP, vol. 7, no. 96, 1958.*

[87] J. M. Luttinger and J. C. Ward, “Ground-state energy of a many-fermion system. II,”

*Phys. Rev., vol. 118, pp. 1417–1427, 1960.*

*[88] A. Klein, “Perturbation theory for an infinite medium of fermions. II,” Phys. Rev.,*
vol. 121, pp. 950–956, 1961.

Bibliography
[89] F. Fuchs, J. Furthmüller, F. Bechstedt, M. Shishkin, and G. Kresse, “Quasiparticle band
*structure based on a generalized Kohn–Sham scheme,” Phys. Rev. B, vol. 76, p. 115109,*
2007.

[90] T. Körzdörfer and N. Marom, “Strategy for finding a reliable starting point for G_{0}W_{0}
*demonstrated for molecules,” Phys. Rev. B, vol. 86, p. 041110, 2012.*

[91] P. Rinke, A. Qteish, J. Neugebauer, and M. Scheffler, “Exciting prospects for solids:

*Exact-exchange based functionals meet quasiparticle energy calculations,” Phys. Status*
*Solidi B, vol. 245, no. 5, pp. 929–945, 2008.*

*[92] I. Shavitt, Methods of Electronic Structure Theory (Modern theoretical chemistry).*

Springer, 1977.

*[93] F. Coester and H. Kümmel, “Short-range correlations in nuclear wave functions,” Nucl.*

*Phys., vol. 17, pp. 477–485, 1960.*

[94] J. Cizek, “On the correlation problem in atomic and molecular systems. Calculation of
wavefunction components in Ursell-type expansion using quantum-field theoretical
*meth-ods,” J. Chem. Phys., vol. 45, pp. 4256–4266, 1966.*

[95] M. Valiev, E. Bylaska, N. Govind, K. Kowalski, T. Straatsma, H. Van Dam, D. Wang,
J. Nieplocha, E. Apra, T. Windus, and W. de Jong, “NWChem: a comprehensive and
*scal-able open-source solution for large scale molecular simulations,” Comput. Phys. Comm.,*
vol. 181, pp. 1477–1489, 2010.

*[96] TURBOMOLE V6.3 2011, a development of University of Karlsruhe and *
*Forschungszen-trum Karlsruhe GmbH, 1989-2007, TURBOMOLE GmbH, since 2007.*

[97] B. Delley, “An all-electron numerical method for solving the local density functional for
*polyatomic molecules,” J. Chem. Phys., vol. 92, pp. 508–517, 1990.*

[98] B. Delley, “From molecules to solids with the DMol^{3}*approach,” J. Chem. Phys., vol. 113,*
pp. 7756–7764, 2000.

[99] V. Blum, R. Gehrke, F. Hanke, P. Havu, V. Havu, X. Ren, K. Reuter, and M. Scheffler,

*“Ab initio molecular simulations with numeric atom-centered orbitals,” Comput. Phys.*

*Commun., vol. 180, pp. 2175–2196, 2009.*

[100] V. Lebedev and D. Laikov, “A quadrature formula for the sphere of the 131st algebraic
*order of accuracy,” Dokl. Math., vol. 59, no. 3, pp. 477–481, 1999.*

*[101] P. P. Ewald, “Die Berechnung optischer und elektrostatischer Gitterpotentiale,” Ann.*

*Phys., vol. 369, no. 3, pp. 253–287, 1921.*

*[102] B. Delley, “Fast calculation of electrostatics in crystals and large molecules,” J. Phys.*

*Chem., vol. 100, pp. 6107–6110, 1996.*

Bibliography
[103] X. Ren, P. Rinke, V. Blum, J. Wieferink, A. Tkatchenko, A. Sanfilippo, K. Reuter, and
M. Scheffler, “Resolution-of-identity approach to Hartree–Fock, hybrid density
*function-als, RPA, MP2 and GW with numeric atom-centered orbital basis functions,” New J.*

*Phys., vol. 14, p. 053020, 2012.*

[104] P. Pulay, “Ab initio calculation of force constants and equilibrium geometries in
*poly-atomic molecules,” Mol. Phys., vol. 18, no. 4, pp. 473–480, 1970.*

*[105] R. Gehrke, First-principles basin-hopping for the structure determination of atomic *
*clus-ters. PhD thesis, Freie Universität Berlin, 2009.*

[106] T. Bredow, G. Geudtner, and K. Jug, “Development of the cyclic cluster approach for
*ionic systems,” J. Comput. Chem., vol. 22, no. 1, pp. 89–101, 2001.*

[107] G. A. Baraff and M. Schlüter, “Self-consistent Green’s-function calculation of the ideal
*Si vacancy,” Phys. Rev. Lett., vol. 41, pp. 892–895, 1978.*

[108] J. Bernholc, N. O. Lipari, and S. T. Pantelides, “Self-consistent method for point defects in
*semiconductors: Application to the vacancy in silicon,” Phys. Rev. Lett., vol. 41, pp. 895–*

899, 1978.

[109] R. Zeller and P. H. Dederichs, “Electronic structure of impurities in Cu, calculated
*self-consistently by Korringa-Kohn-Rostoker Green’s-function method,” Phys. Rev. Lett.,*
vol. 42, pp. 1713–1716, 1979.

[110] F. Beeler, O. K. Andersen, and M. Scheffler, “Theoretical evidence for low-spin ground
*states of early interstitial and late substitutional 3d transition-metal ions in silicon,” Phys.*

*Rev. Lett., vol. 55, pp. 1498–1501, 1985.*

[111] M. Scheffler, C. Droste, A. Fleszar, F. Máca, G. Wachutka, and G. Barzel, “A
*self-consistent surface-Green-function (SSGF) method,” Physica B: Condensed Matter,*
vol. 172, pp. 143–153, 1991.

[112] P. V. Sushko, A. L. Shluger, and C. R. A. Catlow, “Relative energies of surface and
*de-fect states: Ab initio calculations for the MgO (001) surface,” Surf. Sci., vol. 450, no. 3,*
pp. 153–170, 2000.

[113] R. S. Mulliken, “Electronic population analysis on LCAO MO molecular wave functions.

*I,” J. Chem. Phys., vol. 23, pp. 1833–1840, 1955.*

[114] F. L. Hirshfeld, “Bonded-atom fragments for describing molecular charge densities,”

*Theor. Chim. Acta, vol. 44, pp. 129–138, 1977.*

[115] F. Rittner, R. Fink, B. Boddenberg, and V. Staemmler, “Adsorption of nitrogen on rutile
*(110): Ab initio cluster calculations,” Phys. Rev. B, vol. 57, pp. 4160–4171, 1998.*

[116] D. Stodt and C. Hättig, “Embedded cluster density functional and second-order Møller–

Plesset perturbation theory study on the adsorption of N2 *on the rutile (110) surface,” J.*

*Chem. Phys., vol. 137, no. 11, p. 114705, 2012.*

Bibliography
[117] M. J. Puska, S. Pöykkö, M. Pesola, and R. M. Nieminen, “Convergence of supercell
*cal-culations for point defects in semiconductors: Vacancy in silicon,” Phys. Rev. B, vol. 58,*
pp. 1318–1325, 1998.

[118] H.-P. Komsa and A. Pasquarello, “Finite-size supercell correction for charged defects at
*surfaces and interfaces,” Phys. Rev. Lett., vol. 110, p. 095505, 2013.*

[119] S. Lany and A. Zunger, “Accurate prediction of defect properties in density functional
*supercell calculations,” Modell. Simul. Mater. Sci. Eng., vol. 17, no. 8, p. 084002, 2009.*

[120] A. Garcia and J. E. Northrup, “Compensation of p–type doping in ZnSe: the role of
*impurity-native defect complexes,” Phys. Rev. Lett., vol. 74, p. 1131, 1995.*

[121] S. B. Zhang and J. E. Northrup, “Chemical potential dependence of defect formation
*energies in GaAs: Application to Ga self-diffusion,” Phys. Rev. Lett., vol. 67, p. 2339,*
1991.

[122] J. Shim, E. Lee, Y. J. Lee, and R. M. Nieminen, “Density-functional calculations of defect
*formation energies using supercell methods: Defects in diamond,” Phys. Rev. B, vol. 71,*
p. 035206, 2005.

[123] A. Zywietz, J. Furthmüller, and F. Bechstedt, “Vacancies in SiC: influence of Jahn-Teller
*distortions, spin effects, and crystal structure,” Phys. Rev. B, vol. 59, p. 15166, 1999.*

[124] B. Li and H. Metiu, “DFT studies of oxygen vacancies on undoped and doped La_{2}O_{3}
*surfaces,” J. Phys. Chem. C, vol. 114, pp. 12234–12244, 2010.*

[125] Z. Hu and H. Metiu, “Effect of dopants on the energy of oxygen-vacancy formation at the
*surface of ceria: Local or global?,” J. Phys. Chem. C, vol. 115, no. 36, pp. 17898–17909,*
2011.

*[126] L. Vegard, “Die Konstitution der Mischkristalle und die Raumfüllung der Atome,” Z.*

*Phys., vol. 5, no. 1, pp. 17–26, 1921.*

*[127] M. Scheffler, “Lattice relaxations at substitutional impurities in semiconductors,” Physica*
*B+C, vol. 146, pp. 176–186, 1987.*

[128] N. J. Ramer and A. M. Rappe, “Application of a new virtual crystal approach for the study
*of disordered perovskites,” J. Phys. Chem. Solids, vol. 61, pp. 315–320, 2000.*

[129] L. Bellaiche and D. Vanderbilt, “Virtual crystal approximation revisited: Application to
*dielectric and piezoelectric properties of perovskites,” Phys. Rev. B, vol. 61, p. 7877,*
2000.

[130] D. Fritsch, H. Schmidt, and M. Grundmann, “Pseudopotential band structures of rocksalt
MgO, ZnO, and Mg_{1−x}Zn_{x}*O,” Appl. Phys. Lett., vol. 88, no. 13, p. 134104, 2006.*

[131] M. Casarin, C. Maccato, and A. Vittadini, “Electronic structure of Nb impurities in and
on TiO_{2}*,” Phys. Chem. Chem. Phys., vol. 1, pp. 3793–3799, 1999.*

Bibliography
[132] J. Sauer and M. Sierka, “Combining quantum mechanics and interatomic potential
*func-tions in ab initio studies of extended systems,” J. Comput. Chem., vol. 21, no. 16,*
pp. 1470–1493, 2000.

[133] E. Kaxiras, Y. Bar-Yam, J. D. Joannopoulos, and K. C. Pandey, “Ab initio theory of polar semiconductor surfaces. I. Methodology and the (2×2) reconstructions of GaAs(111),”

*Phys. Rev. B, vol. 35, no. 18, pp. 9625–9635, 1987.*

*[134] M. Scheffler, “Thermodynamic aspects of bulk and surface defects,” Stud. Surf. Sci.*

*Catal., vol. 40, pp. 115–122, 1988.*

[135] K. Reuter, C. Stampfl, and M. Scheffler, “Ab initio thermodynamics and statistical
*me-chanics of surface properties and functions,” in Handbook of Materials Modeling, Part A.*

*Methods (S. Yip, ed.), Springer, 2005.*

*[136] D. A. Mc Quarrie, Statistical Mechanics. Harper and Row, New York, 1976.*

[137] M. Ernzerhof, J. P. Perdew, and K. Burke, “Coupling-constant dependence of atomization
*energies,” Int. J. Quantum Chem., vol. 64, no. 3, pp. 285–295, 1997.*

*[138] A. Gross, Theoretical Surface Science: A Microscopic Perspective. Springer, 2009.*

[139] D. Feller and K. A. Peterson, “Re-examination of atomization energies for the Gaussian-2
*set of molecules,” J. Chem. Phys., vol. 110, no. 17, pp. 8384–8396, 1999.*

*[140] D. Stull and P. H., JANAF Thermochemical Tables, 2nd edn. U.S. National Bureau of*
Standards, Washington, D.C., 1971.

*[141] N. W. Ashcroft and N. D. Mermin, Solid State Physics. CBS Publishing, Tokyo, 1981.*

[142] A. Togo, F. Oba, and I. Tanaka, “First-principles calculations of the ferroelastic
transi-tion between rutile-type and CaCl_{2}-type SiO_{2} *at high pressures,” Phys. Rev. B, vol. 78,*
p. 134106, 2008.

[143] M. Leslie and N. J. Gillan, “The energy and elastic dipole tensor of defects in ionic
*crys-tals calculated by the supercell method,” J. Phys. C, vol. 18, pp. 973–982, 1985.*

[144] J. Lento, J. Mozos, and R. Nieminen, “Charged point defects in semiconductors and the
*supercell approximation,” J. Phys.: Condens. Mat., vol. 14, no. 10, pp. 2637–2645, 2002.*

[145] D. Segev and S. Wei, “Design of shallow donor levels in diamond by isovalent-donor
*coupling,” Phys. Rev. Lett., vol. 91, no. 12, p. 126406, 2003.*

[146] C. G. Van de Walle, “First-principles calculations for defects and impurities: Applications
*to III-nitrides,” J. Appl. Phys., vol. 95, no. 8, p. 3851, 2004.*

*[147] P. A. Schultz, “Theory of defect levels and the "Band gap problem" in silicon,” Phys. Rev.*

*Lett., vol. 96, p. 246401, 2006.*